LMucko/crystallography-open-database huggingface dataset:
Ca-substitution and O-doping effects in superconducting Cu (Ba0.8 Sr0.2)2 (Yb1-x Cax) Cu2 O6+z obtained from neutron diffraction refinements
Karppinen, M.; Yamauchi, H.; Rundloef, H.; Nakane, T.; Fujinami, K.; Peitola, K.; Tellgren, R.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 60 (1999) 4378–4385; doi:

data_1521378
_publ_section_title
;
 Ca-substitution and O-doping effects in superconducting Cu (Ba0.8 Sr0.2)2
 (Yb1-x Cax) Cu2 O6+z obtained from neutron diffraction refinements
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              4378
_journal_page_last               4385
_journal_volume                  60
_journal_year                    1999
_chemical_formula_sum            'Ba1.6 Ca0.35 Cu3 O6.075 Sr0.4 Yb0.65'
_chemical_name_systematic
'Cu (Ba0.8 Sr0.2)2 (Yb0.65 Ca0.35) Cu2 O6.075'
_space_group_IT_number           123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.8334
_cell_length_b                   3.8334
_cell_length_c                   11.734
_cell_volume                     172.431
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            Karppinen_PRBMDO_1999_714.cif
_cod_data_source_block           Ba1.6Ca0.35Cu3O6.075Sr0.4Yb0.65
_cod_original_cell_volume        172.4306
_cod_database_code               1521378
Ca-substitution and O-doping effects in superconducting Cu (Ba0.8 Sr0.2)2 (Yb1-x Cax) Cu2 O6+z obtained from neutron diffraction refinements
Karppinen, M.; Yamauchi, H.; Fujinami, K.; Nakane, T.; Rundloef, H.; Peitola, K.; Tellgren, R.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 60 (1999) 4378–4385; doi:

data_1521379
_publ_section_title
;
 Ca-substitution and O-doping effects in superconducting Cu (Ba0.8 Sr0.2)2
 (Yb1-x Cax) Cu2 O6+z obtained from neutron diffraction refinements
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              4378
_journal_page_last               4385
_journal_volume                  60
_journal_year                    1999
_chemical_formula_sum            'Ba1.6 Cu3 O6.201 Sr0.4 Yb'
_chemical_name_systematic        'Cu (Ba0.8 Sr0.2)2 Yb Cu2 O6.201'
_space_group_IT_number           123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.8342
_cell_length_b                   3.8342
_cell_length_c                   11.743
_cell_volume                     172.635
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            Karppinen_PRBMDO_1999_715.cif
_cod_data_source_block           Ba1.6Cu3O6.201Sr0.4Yb1
_cod_original_cell_volume        172.6349
_cod_original_formula_sum        'Ba1.6 Cu3 O6.201 Sr0.4 Yb1'
_cod_database_code               1521379
Ca-substitution and O-doping effects in superconducting Cu (Ba0.8 Sr0.2)2 (Yb1-x Cax) Cu2 O6+z obtained from neutron diffraction refinements
Karppinen, M.; Fujinami, K.; Yamauchi, H.; Nakane, T.; Peitola, K.; Rundloef, H.; Tellgren, R.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 60 (1999) 4378–4385; doi:

data_1521380
_publ_section_title
;
 Ca-substitution and O-doping effects in superconducting Cu (Ba0.8 Sr0.2)2
 (Yb1-x Cax) Cu2 O6+z obtained from neutron diffraction refinements
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              4378
_journal_page_last               4385
_journal_volume                  60
_journal_year                    1999
_chemical_formula_sum            'Ba1.6 Cu3 O6.35 Sr0.4 Yb'
_chemical_name_systematic        'Cu (Ba0.8 Sr0.2)2 Yb Cu2 O6.35'
_space_group_IT_number           47
_symmetry_space_group_name_Hall  '-P 2 2'
_symmetry_space_group_name_H-M   'P m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.8172
_cell_length_b                   3.8465
_cell_length_c                   11.667
_cell_volume                     171.305
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            Karppinen_PRBMDO_1999_716.cif
_cod_data_source_block           Ba1.6Cu3O6.35Sr0.4Yb1
_cod_original_cell_volume        171.3049
_cod_original_formula_sum        'Ba1.6 Cu3 O6.35 Sr0.4 Yb1'
_cod_database_code               1521380
Ca-substitution and O-doping effects in superconducting Cu (Ba0.8 Sr0.2)2 (Yb1-x Cax) Cu2 O6+z obtained from neutron diffraction refinements
Karppinen, M.; Yamauchi, H.; Nakane, T.; Fujinami, K.; Tellgren, R.; Peitola, K.; Rundloef, H.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 60 (1999) 4378–4385; doi:

data_1521381
_publ_section_title
;
 Ca-substitution and O-doping effects in superconducting Cu (Ba0.8 Sr0.2)2
 (Yb1-x Cax) Cu2 O6+z obtained from neutron diffraction refinements
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              4378
_journal_page_last               4385
_journal_volume                  60
_journal_year                    1999
_chemical_formula_sum            'Ba1.6 Cu3 O6.817 Sr0.4 Yb'
_chemical_name_systematic        'Cu (Ba0.8 Sr0.2)2 Yb Cu2 O6.817'
_space_group_IT_number           47
_symmetry_space_group_name_Hall  '-P 2 2'
_symmetry_space_group_name_H-M   'P m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.804
_cell_length_b                   3.8583
_cell_length_c                   11.637
_cell_volume                     170.796
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            Karppinen_PRBMDO_1999_717.cif
_cod_data_source_block           Ba1.6Cu3O6.817Sr0.4Yb1
_cod_original_cell_volume        170.7959
_cod_original_formula_sum        'Ba1.6 Cu3 O6.817 Sr0.4 Yb1'
_cod_database_code               1521381
Ca-substitution and O-doping effects in superconducting Cu (Ba0.8 Sr0.2)2 (Yb1-x Cax) Cu2 O6+z obtained from neutron diffraction refinements
Karppinen, M.; Yamauchi, H.; Rundloef, H.; Fujinami, K.; Peitola, K.; Nakane, T.; Tellgren, R.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 60 (1999) 4378–4385; doi:

data_1521382
_publ_section_title
;
 Ca-substitution and O-doping effects in superconducting Cu (Ba0.8 Sr0.2)2
 (Yb1-x Cax) Cu2 O6+z obtained from neutron diffraction refinements
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              4378
_journal_page_last               4385
_journal_volume                  60
_journal_year                    1999
_chemical_formula_sum            'Ba1.6 Cu3 O6.999 Sr0.4 Yb'
_chemical_name_systematic        'Cu (Ba0.8 Sr0.2)2 Yb Cu2 O6.999'
_space_group_IT_number           47
_symmetry_space_group_name_Hall  '-P 2 2'
_symmetry_space_group_name_H-M   'P m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.7934
_cell_length_b                   3.8615
_cell_length_c                   11.614
_cell_volume                     170.124
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            Karppinen_PRBMDO_1999_718.cif
_cod_data_source_block           Ba1.6Cu3O6.999Sr0.4Yb1
_cod_original_cell_volume        170.1244
_cod_original_formula_sum        'Ba1.6 Cu3 O6.999 Sr0.4 Yb1'
_cod_database_code               1521382
Darstellung und Kristallstruktur von A Ni10 P3 (A: Zn, Ga, Sn, Sb)
Keimes, V.; Blume, H.M.; Mewis, A.; Zeitschrift fuer Anorganische und Allgemeine Chemie 625 (1999) 207–210; doi:

data_1521383
_publ_section_title
;
 Darstellung und Kristallstruktur von A Ni10 P3 (A: Zn, Ga, Sn, Sb)
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              207
_journal_page_last               210
_journal_volume                  625
_journal_year                    1999
_chemical_formula_sum            'Ni10 P3 Zn'
_chemical_name_systematic        'Zn Ni10 P3'
_space_group_IT_number           164
_symmetry_space_group_name_Hall  '-P 3 2"'
_symmetry_space_group_name_H-M   'P -3 m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   7.665
_cell_length_b                   7.665
_cell_length_c                   9.36
_cell_volume                     476.245
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Keimes_ZAACAB_1999_847.cif
_cod_data_source_block           Ni10P3Zn1
_cod_original_cell_volume        476.2454
_cod_original_formula_sum        'Ni10 P3 Zn1'
_cod_database_code               1521383
Darstellung und Kristallstruktur von A Ni10 P3 (A: Zn, Ga, Sn, Sb)
Keimes, V.; Blume, H.M.; Mewis, A.; Zeitschrift fuer Anorganische und Allgemeine Chemie 625 (1999) 207–210; doi:

data_1521384
_publ_section_title
;
 Darstellung und Kristallstruktur von A Ni10 P3 (A: Zn, Ga, Sn, Sb)
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              207
_journal_page_last               210
_journal_volume                  625
_journal_year                    1999
_chemical_formula_sum            'Ni10 P3 Sn'
_chemical_name_systematic        'Sn Ni10 P3'
_space_group_IT_number           164
_symmetry_space_group_name_Hall  '-P 3 2"'
_symmetry_space_group_name_H-M   'P -3 m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   7.674
_cell_length_b                   7.674
_cell_length_c                   9.621
_cell_volume                     490.676
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Keimes_ZAACAB_1999_848.cif
_cod_data_source_block           Ni10P3Sn1
_cod_original_cell_volume        490.6756
_cod_original_formula_sum        'Ni10 P3 Sn1'
_cod_database_code               1521384
Powder neutron diffraction study of the high temperature phase transitions in Na Ta O3
Kennedy, B.J.; Prodjosantoso, A.K.; Howard, C.J.; Journal of Physics: Condensed Matter 11 (1999) 6319–6327; doi:

data_1521385
_publ_section_title
;
 Powder neutron diffraction study of the high temperature phase
 transitions in Na Ta O3
;
_journal_name_full               'Journal of Physics: Condensed Matter'
_journal_page_first              6319
_journal_page_last               6327
_journal_volume                  11
_journal_year                    1999
_chemical_formula_sum            'Na O3 Ta'
_chemical_name_systematic        'Na (Ta O3)'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.4768
_cell_length_b                   5.5212
_cell_length_c                   7.789
_cell_volume                     235.528
_citation_journal_id_ASTM        JCOMEL
_cod_data_source_file            Kennedy_JCOMEL_1999_101.cif
_cod_data_source_block           Na1O3Ta1
_cod_original_cell_volume        235.5277
_cod_original_sg_symbol_Hall     '-P 2ac 2n (z,x,y)'
_cod_original_formula_sum        'Na1 O3 Ta1'
_cod_database_code               1521385
Powder neutron diffraction study of the high temperature phase transitions in Na Ta O3
Kennedy, B.J.; Prodjosantoso, A.K.; Howard, C.J.; Journal of Physics: Condensed Matter 11 (1999) 6319–6327; doi:

data_1521386
_publ_section_title
;
 Powder neutron diffraction study of the high temperature phase
 transitions in Na Ta O3
;
_journal_name_full               'Journal of Physics: Condensed Matter'
_journal_page_first              6319
_journal_page_last               6327
_journal_volume                  11
_journal_year                    1999
_chemical_formula_sum            'Na O3 Ta'
_chemical_name_systematic        'Na (Ta O3)'
_space_group_IT_number           127
_symmetry_space_group_name_Hall  '-P 4 2ab'
_symmetry_space_group_name_H-M   'P 4/m b m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.5503
_cell_length_b                   5.5503
_cell_length_c                   3.9335
_cell_volume                     121.175
_citation_journal_id_ASTM        JCOMEL
_cod_data_source_file            Kennedy_JCOMEL_1999_102.cif
_cod_data_source_block           Na1O3Ta1
_cod_original_cell_volume        121.1747
_cod_original_formula_sum        'Na1 O3 Ta1'
_cod_database_code               1521386
High-temperature phase transitions in Sr Zr O3
Kennedy, B.J.; Howard, C.J.; Chakoumakos, B.C.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 59 (1999) 4023–4027; doi:

data_1521387
_publ_section_title
;
 High-temperature phase transitions in Sr Zr O3
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              4023
_journal_page_last               4027
_journal_volume                  59
_journal_year                    1999
_chemical_formula_sum            'O3 Sr Zr'
_chemical_name_systematic        'Sr (Zr O3)'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.9763
_cell_length_b                   5.8171
_cell_length_c                   8.2048
_cell_volume                     285.238
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            Kennedy_PRBMDO_1999_696.cif
_cod_data_source_block           O3Sr1Zr1
_cod_original_cell_volume        285.2377
_cod_original_sg_symbol_Hall     '-P 2ac 2n (z,x,y)'
_cod_original_formula_sum        'O3 Sr1 Zr1'
_cod_database_code               1521387
High-temperature phase transitions in Sr Zr O3
Kennedy, B.J.; Howard, C.J.; Chakoumakos, B.C.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 59 (1999) 4023–4027; doi:

data_1521388
_publ_section_title
;
 High-temperature phase transitions in Sr Zr O3
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              4023
_journal_page_last               4027
_journal_volume                  59
_journal_year                    1999
_chemical_formula_sum            'O3 Sr Zr'
_chemical_name_systematic        'Sr (Zr O3)'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.27
_cell_length_b                   8.2732
_cell_length_c                   8.2586
_cell_volume                     565.048
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            Kennedy_PRBMDO_1999_697.cif
_cod_data_source_block           O3Sr1Zr1
_cod_original_cell_volume        565.0482
_cod_original_formula_sum        'O3 Sr1 Zr1'
_cod_database_code               1521388
High-temperature phase transitions in Sr Zr O3
Kennedy, B.J.; Howard, C.J.; Chakoumakos, B.C.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 59 (1999) 4023–4027; doi:

data_1521389
_publ_section_title
;
 High-temperature phase transitions in Sr Zr O3
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              4023
_journal_page_last               4027
_journal_volume                  59
_journal_year                    1999
_chemical_formula_sum            'O3 Sr Zr'
_chemical_name_systematic        'Sr (Zr O3)'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.1514
_cell_length_b                   4.1514
_cell_length_c                   4.1514
_cell_volume                     71.546
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            Kennedy_PRBMDO_1999_701.cif
_cod_data_source_block           O3Sr1Zr1
_cod_original_cell_volume        71.54574
_cod_original_formula_sum        'O3 Sr1 Zr1'
_cod_database_code               1521389
High-temperature phase transitions in Sr Hf O3
Kennedy, B.J.; Howard, C.J.; Chakoumakos, B.C.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 60 (1999) 2972–2975; doi:

data_1521390
_publ_section_title
;
 High-temperature phase transitions in Sr Hf O3
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              2972
_journal_page_last               2975
_journal_volume                  60
_journal_year                    1999
_chemical_formula_sum            'Hf O3 Sr'
_chemical_name_systematic        'Sr (Hf O3)'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.7516
_cell_length_b                   5.7646
_cell_length_c                   8.1344
_cell_volume                     269.702
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            Kennedy_PRBMDO_1999_707.cif
_cod_data_source_block           Hf1O3Sr1
_cod_original_cell_volume        269.7015
_cod_original_sg_symbol_Hall     '-P 2ac 2n (z,x,y)'
_cod_original_formula_sum        'Hf1 O3 Sr1'
_cod_database_code               1521390
High-temperature phase transitions in Sr Hf O3
Kennedy, B.J.; Howard, C.J.; Chakoumakos, B.C.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 60 (1999) 2972–2975; doi:

data_1521391
_publ_section_title
;
 High-temperature phase transitions in Sr Hf O3
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              2972
_journal_page_last               2975
_journal_volume                  60
_journal_year                    1999
_chemical_formula_sum            'Hf O3 Sr'
_chemical_name_systematic        'Sr (Hf O3)'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.1741
_cell_length_b                   8.1974
_cell_length_c                   8.1797
_cell_volume                     548.092
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            Kennedy_PRBMDO_1999_708.cif
_cod_data_source_block           Hf1O3Sr1
_cod_original_formula_sum        'Hf1 O3 Sr1'
_cod_database_code               1521391
High-temperature phase transitions in Sr Hf O3
Kennedy, B.J.; Howard, C.J.; Chakoumakos, B.C.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 60 (1999) 2972–2975; doi:

data_1521392
_publ_section_title
;
 High-temperature phase transitions in Sr Hf O3
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              2972
_journal_page_last               2975
_journal_volume                  60
_journal_year                    1999
_chemical_formula_sum            'Hf O3 Sr'
_chemical_name_systematic        'Sr (Hf O3)'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.1138
_cell_length_b                   4.1138
_cell_length_c                   4.1138
_cell_volume                     69.619
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            Kennedy_PRBMDO_1999_710.cif
_cod_data_source_block           Hf1O3Sr1
_cod_original_cell_volume        69.61928
_cod_original_formula_sum        'Hf1 O3 Sr1'
_cod_database_code               1521392
Kristallstrukturen der Monofluorosulfite M S O2 F (M = K, Rb)
Kessler, U.; Jansen, M.; Zeitschrift fuer Anorganische und Allgemeine Chemie 625 (1999) 385–388; doi:

data_1521393
_publ_section_title
;
 Kristallstrukturen der Monofluorosulfite M S O2 F (M = K, Rb)
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              385
_journal_page_last               388
_journal_volume                  625
_journal_year                    1999
_chemical_formula_sum            'F K O2 S'
_chemical_name_systematic        'K (S O2 F)'
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.73
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   6.962
_cell_length_b                   5.663
_cell_length_c                   4.658
_cell_volume                     174.923
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Kessler_ZAACAB_1999_872.cif
_cod_data_source_block           F1K1O2S1
_cod_original_cell_volume        174.9226
_cod_original_formula_sum        'F1 K1 O2 S1'
_cod_database_code               1521393
Kristallstrukturen der Monofluorosulfite M S O2 F (M = K, Rb)
Kessler, U.; Jansen, M.; Zeitschrift fuer Anorganische und Allgemeine Chemie 625 (1999) 385–388; doi:

data_1521394
_publ_section_title
;
 Kristallstrukturen der Monofluorosulfite M S O2 F (M = K, Rb)
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              385
_journal_page_last               388
_journal_volume                  625
_journal_year                    1999
_chemical_formula_sum            'F O2 Rb S'
_chemical_name_systematic        'Rb (S O2 F)'
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.14
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.172
_cell_length_b                   5.867
_cell_length_c                   4.84
_cell_volume                     194.613
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Kessler_ZAACAB_1999_873.cif
_cod_data_source_block           F1O2Rb1S1
_cod_original_cell_volume        194.6132
_cod_original_formula_sum        'F1 O2 Rb1 S1'
_cod_database_code               1521394